Jurnal Teknologi, 43(A) Dis. 2006: 11–20 © Universiti Teknologi Malaysia
Unit Kejuruteraan Kualiti, Jabatan Kejuruteraan Pengeluaran & Industri, Fakulti Kejuruteraan Mekanikal, Universiti Teknologi Malaysia, 81300 Skudai, Johor.
* Corresponding author: Email: firstname.lastname@example.org
OPTIMIZATION OF SOLDER PASTE PRINTING PARAMETERS USING DESIGN OF EXPERIMENTS (DOE)
SEKHARAN GOPAL1, JAFRI MOHD ROHANI2*, SHA’RI MOHD YUSOF3 &
ZAILIS ABU BAKAR4
Abstract. The solder paste printing process is an important process in the assembly of Surface Mount Technology (SMT) devices using the reflow soldering technique. There is a wide agreement in the industry that the paste printing process accounts for the majority of assembly defects. Experience with this process has shown that typically over 60% of all soldering defects are due to problems associated with the screening process. Therefore, operation and parameter setup of the stencil printing process are the key elements when trying to minimize defects. Parameters such as squeegee pressure, squeegee speed, stencil separation speed, snap-off and stencil cleaning interval are the most important factors in the process to achieve a better yield. This paper describes the experiment design approach for solder paste printing process. A factorial design technique has been used to study the effects of the solder paste printing process parameters. Sixteen experimental trial were carried out in the experiment with two levels for each factor. The output from the experiment is the solder paste height, and the data has been statistically analyzed by using Minitab Software. The Analysis of Variance (ANOVA) showed that the important factors for the solder paste height are squeegee pressure and snap-off with the optimal setting for printing speed, squeegee pressure, snap-off, squeegee separation, and cleaning interval. The experiment error between the predicted regression model and actual verification was found to be 1.61%. It is shown that by using DOE 18% improvement of the solder paste height can be achieved.
Keywords: Design of experiments, solder paste printing, Analysis of Variance (ANOVA), regression analysis
varians menunjukkan bahawa faktor yang penting bagi ketinggian percetakan timah ialah tekanan
squeegee dan snap-off dengan menetapkan kelajuan percetakan, tekanan squeegee, snap-off, pengasingan squeegee dan sela pembersihan pada tahap optimum. Ralat eksperimen antara model regrasi dan pengesahan sebenar ialah sebanyak 1.61% Penggunaan DOE menunjukkan 18% pembaikan ketinggian pencetakan timah boleh dicapai.
Kata kunci: Reka bentuk eksperimen, pencetak timah, analisa varians, analisa regrasi 1.0 INTRODUCTION
2.0 DETAILS OF PROCESS PARAMETERS 2.1 Stencil
Metal stencils can be made of different materials. Besides stainless steel, they can be made of copper, bronze, or nickel. There are 3 different metal stencil-manufacturing methods: Etching, electroforming and laser cutting. The apertures in both laser-cut and electroformed stencils have very sharp edges and are slightly conic. This makes the solder paste slip easily off the aperture edges and thereby secures a uniform print. The metal stencils are attached to the printing frame using tensioned mesh or directly using a special frame with gripping systems, which can easily damage the stencils and thereby resulting in poor printing quality. The thickness of the metal stencil is typically 150 microns but 100, 125 and 200 microns are also available. The thickness should be chosen based on the job in hand. For very fine pitch such as 0.3 mm lead pitch, 100 or 125-micron stencils could be used and for lead pitch down to 0.5 mm, 150-micron stencils can be used. The stencil thickness together with the aperture size also determines the amount of solder paste present to form each solder joint during reflow soldering. As a guideline, the minimum stencil aperture width must be at least 3 times (preferable 5 times) the diameter of the largest solder particle and the stencil aperture width should also be larger than the stencil thickness. Rounded aperture corners will reduce clogging of fine pitch apertures and smearing. The top surface of the metal stencil should be slightly roughened to achieve a perfect solder paste roll during printing.
Dust and dirt from the air that ends up on the PCBs and stencils can cause defects such as bridging and poor wet-ability in the reflow soldering process. A small piece of fibre or hair between two fine pitch solder pads can easily cause bridging. It is therefore very important that the PCBs are stored in sealed packages and if necessary, cleaned before use. Air draught in the production area can speed up evaporation of the solvents in the solder paste and thereby makes the solder paste dry out. High temperature can also make the solder paste dry out quickly. If the room temperature in the production area varies a lot, it will be very difficult to control the printing process. The viscosity of the solder paste changes with the temperature and the solder paste print will sometimes be perfected and at other times, paste will slump and result in bridging. The temperature window is between 21 – 25°C.
2.3 Solder Paste
2.4 Stencil Printing Parameters
Stencil Printing Parameters are the most important factors in the solder paste printing process to achieve better yield. The first parameter is the squeegee pressure. It should be as low as possible to scrape the stencil clean of solder paste particles when printing. The amount of pressure is determined by the printing speed and stencil type. The printing speed is usually recommended by paste manufacturer.
Usually the solder paste manufacturer only gives guideline to the right printing speed: typically between 20 and 80 mm per second. The printing speed is a major factor in the printing cycle time and therefore, important as it can compromise the print quality. Snap off is the distance between the stencil underside and the PCB placed in print position but without the squeegee touching the stencil. For metal stencil printing, the snap off should be zero and also called contact printing. For mesh screen-printing, the snap off should be set to between 0.5 and 3.0 mm. A high snap off will result in a thicker layer of solder paste. The speed of separation between stencil and PCB after printing is important. A too rapid separation speed when printing fine pitch will result in clogging of the stencil apertures. It will also result in tailing and formation high of edges around the solder paste deposits. In general, if all printing parameters are in control, stencil underside cleaning is not necessary. Cleaning can be done either manually or automatically. The wiper does not clean the stencils underside but simply move the solder paste particles from around the apertures to the complete stencils underside. Stencil cleaning prior to use is important to prevent dust and dirt from entering the solder joints.
3.0 EXPERIMENT DESIGN AND RESULT ANALYSIS 3.1 Experimental Design Steps
both the average amount of solder paste applied and the process variability. This cross-functional team selected five factors for the screening experiment. They also decided to use two levels for each factor. The five factors chosen and their actual low and high levels are as follows:
A – Squeegee pressure; levels (4 and 7 kg). B – Squeegee speed; levels (30 and 60 mm/s). C – Snap off; levels (–0.1 and 0.1 mm). D – Separation speed; levels (1 and 5 mm/s). E – Cleaning internal (Stroke) (5 and 10)
The team also identified two potential nuisance factors; temperature and humidity. It was felt that large variation in these factors could potentially adversely affect the experimental results. Therefore, the team decided to hold these factors constant during the experiment. Although the factors are controlled, the team directed close attention to the results for any potential influence. The response is the height of solder paste. The experimental design selected was a one-half fraction of a 25–1 design. The defining relation for this design is I = ABCDE. Consequently, every main effect is aliased with a four-factor interaction, and every two-factor interaction is aliased with three-factor interaction. Thus, the design is of resolution V. The design provides good information concerning the main effects and two-factor interactions.
3.2 Data Analysis
The results of the experiments are analysed in the following section.
3.2.1 Analysis of Variance (ANOVA)
The following section describes the results for the dependent variable (response) solder paste height in mils. The analysis performed is an Analysis of Variance “ANOVA” Model that identifies the amount of experimental error and the significance of the model in accounting for the variability in the experiment. The test identifies the factors and interactions that are significant. Effect listed as “most significant” represent the independent process variables that have the greatest influence on a particular treatment response. The important factors are graphically displayed using main effect plots, such as effect pareto on solder paste height and interaction plots (Figures 1 and 2).
Figure 1 Effect pareto on solder paste height
Figure 2 Interaction plot for solder paste height
-1 1 -1 1 -1 1 -1 1
6.00 6.25 6.50 6.00 6.25 6.50 6.00 6.25 6.50 6.00 6.25 6.50
Cleaning interval Interaction plot (data means) for SolderHt
0 1 2 3 4 5 6
D A AE BE E BD AD C B DE AB CD
Pareto chart of the standardized effects (response is SolderHt, Alpha = .10)
A: Print speed B: Squegee pressure C: Snap-off
Any effect that extends past the reference line is considered significant. The 3 largest dominant factors are:
(i) CD Interaction: Snap off × Separation speed (ii) AB Interaction: Print speed × Squeegee pressure (iii) DE Interaction: Separation speed × Cleaning interval
Interaction plot was used to determine if two factors interact in their effect on the response and compare the relative strength of the effects. An analysis of variance (ANOVA) conducted for the response of the parameters, provided assurance that each of the initially selected effects was statistically significant. In some cases, a variable was not significant at the traditional 0.05 level, but was retained in the model because it was involved in an interaction. Figure 2 summarizes the results from the ANOVA where cells containing the symbol “1” identify factors having the strongest effects and cells containing the symbol “5” identify factors having the smallest effects. The normal probability plots of residual for each response is satisfactory. From the main effect plot, the optimal parameters to a better solder paste height parameters for each factor may be known. For the response solder paste height, the smallest value is considered as the best result.
3.3 Optimal Setting
From the data that has been analyzed, the optimal setting for solder paste printing process was obtained. The optimal setting was as follows:
A – Printing speed (60 mm/s). B – Squeegee pressure (7 kg). C – Snap off (–0.1 mm).
D – Separation speed ( 1 mm/s). E – Cleaning internal (5 Internal).
3.4 Verification and Validity
For verification experiment, five runs were carried out. So, there are five replication for this verification experiment. The response solder paste height of the verification experiment was also measured by using the Cyberoptics Cyberscan 200. After the measurement, the resulted solder paste height was collected and shown in Table 1.
% of error is small, this result is valid. The optimize setting can be used to the solder paste printing process for the model SB0350. To calculate the percentage of improvement, first five solder paste thickness data before the experiment were chosen. Then, the average of the data was calculated. The data that has been chosen are shown in Table 2.
From Table 2, the average of the five worst flatness data from the experiment result is 6.75 mils. So the percent improvement can be calculated as:
% improvement = [(6.78 – 5.68) / 5.68] × 100 % = 18 %
This paper has discussed an application of the Design of Experiment (DOE) ½ fraction for optimizing the solder paste printing process. Fractional factorial designs are useful in factor screening because they reduce the number of runs to a manageable
Table 1 Result of verification experiment for
response solder paste height
Table 2 Five worst data of solder paste height
from experiment result (Response - solder paste, height (mm))
size. The runs that are performed are a selected or fraction of the full factorial design. As shown in this study, the DOE are often carried out in four phases: planning, screening (also called process characterization), optimization, and verification. Well-designed experiments can produce significantly more information and often require fewer runs than haphazard or unplanned experiments. In addition, a well-designed experiment will ensure that we can evaluate the effects that have been identified as important. In this case study, we can summarized that the DOE provides a systematic and efficient methodology for design optimization of the solder paste printing process with far less effort than would be required for most optimization techniques. At the end of this study, it was found the optimal setting for solder paste printing process are high squeegee pressure, high printing speed, low snap-off, low separation speed and low cleaning interval. These optimal setting results in a small value of response solder paste height after the verification run was conducted. It was found that the percentage between the predicted and actual experiment is 1.16%. This is very small and so the experiment is considered valid. From calculation, it was found that, by using the classical method of DOE, 20% improvement was achieved. The cycle time for the printing process can also be minimized by increasing of the speed of separation and maximizing the cleaning interval.
 Burr, D. C. 1999. Solder Paste Printing Guidelines for BGA and CSP Assemblies. SMT Magazine, January 1999. 70-72.
 Lo, E. K., N. N. Ekere, and S. H. Mannan. 1993. The Future of Solder Paste Printing for SMT Reflow Soldering. Soldering and Surface Mount Technology Journal. 13: 22-25.
 Currie, M. 1996. Modeling of the Paste Withdrawal Sub-Process in the Stencil Printing of Solder Pastes for the Reflow Soldering of Surface Mount Assemblies. University of Salford.
 Danielsson, H. 1995. Surface Mount Technology with Fine Pitch Components. Chapman and Hall.  Haslehurst, L., and N. N. Ekere. 1996. Parameter Interactions in Stencil Printing of Solder Paste. Journal
of Electronics Manufacturing. 6(4): 307-316.
 Ekere, N. N., E. K. Lo, and L. Ismail. 1993. Experiment Study of Stencil-substrate Separation Speed in Solder Paste Printing for Reflow Soldering. Journal of Electronics Manufacturing. 3(4): 25-9.
 Mannan, S. H., and N. N. Ekere. 1993. Predicting Scooping and Skipping in Solder Paste Printing for Reflow Soldering of SMT Devices. Soldering and Surface Mount Technology Journal. 15: 14-17.
 Xiao, M., K. J. Lawless, and N. C. Lee. 1993. Prospects of Solder Paste in Ultra Fine Pitch Era. Soldering and Surface Mount Technology. 5-14.
 Hwang, J. S. 1989. Solder Paste in Electronics Packaging: Technology and Applications in Surface Mount, Hybrid Circuits and Components Assembly. New York NY: Van Nostrand Reinhold.
 Hwang, J. S. 1994. Solder/screen printing. Surface Mount Technology. 44-50.
 Ismail, L., S. H. Mannan, N. N. Ekere, and E. K. Lo. 1993. Experiment Study of the Printing of Solder Paste Using the Metal Blade Squeegee System. Proceedings of the 30th International MATADOR Conference, Manchester. 263-6.
 Lau, J., and C. Chang. 2000. Taguchi Design of Experiment of Wafer Bumping by Stencil Printing.
Electronic Component and Technology Conference.
 Ekere, N. N., E. K. Lo, and Mannan, S. H. 1994. Process Modeling Mmaps for Solder Paste Printing.
 Butlars, S. K. 1993. Parameters of Solder Paste Printing for Fine Pitch Components. Proceedings NEPCON-WEST ’93. 1254-65
 Morris, J. R., and T. Wojcik. 1990. Stencil Printing of Solder Paste for Fine-pitch Surface Mount Assembly.
Soldering & Surface Mount Technology. 5: 10-14.
 Derringer, G., and R. Strich. 1980. Simultaneous Optimization of Several Response Variables. Journal of Quality Technology. 12(4): 214-19.
 Anderson, V. L., and R. A. McLean. 1974. Design of Experiments-A Realistic Approach. Marcel Dekker, Inc.
 Kempthorne, O. 1973. Design and Analysis of Experiments. Robert E. Krieger Publishing Company.  Montgomery, D. C. 1976. Design and Analysis of Experiments. New York, NY: John Wiley and Sons.  Montgomery, D. C. 1991. Design and Analysis of Experiments, Third Edition. New York, NY: John Wiley
 Montgomery, D. C. 1997. Design and Analysis of Experiments, 4th ed. New York, NY: Wiley.